novel polymer design for radiation ?· novel polymer design for radiation curable psas ming zhao,...
Post on 30-Aug-2018
Embed Size (px)
NOVEL POLYMER DESIGN FOR RADIATION CURABLE PSAS
Ming Zhao, Victor Lu, Leo Ternorutsky, Patrice Mariucci, Sarah Shinkwin, Mark Jason, Jong Guo, and Morris Bingham Cytec Specialty Chemicals, Pressure Sensitive Adhesives R&D, Springfield, MA USA Abstract A new acrylic urethane polymer, comprised of a unique mixture of structurally different polyols and isocyanates, provides significant improvement in the high temperature performance of pressure sensitive adhesives. This new polymer, in combination with other functional monomers and oligomers, can be formulated with various tackifiers and other additives to provide a solvent-free and radiation curable product that offers tack, adhesion and high temperature cohesive strength when applied to high surface energy substrates (stainless steel) as well as low (polypropylene). The invented technology targets primarily the high performance tape market. Introduction UV-cure technology in pressure sensitive adhesives (PSAs) became actively pursued in the early 70s. Since that time, different types of polymerizations initiated by UV energy have been developed that include the cross-linking of acrylic syrups, building the photoinitiators on the polymer chain, and the cationic cure of epoxy-functional block copolymers. These technologies have attracted the attention of the PSA market because of three major advantages relative to traditional waterborne and solventborne products: lower converting costs, flexible processing, and environmental friendliness. Moreover, these UV-cure technologies can also offer significant performance improvements in comparison with waterborne and solventborne products. However, like any technology, these UV-curable PSAs have encountered their own technical and financial challenges: 1. the capability to provide good adhesion to both low and high surface energy substrates; 2. simultaneously exhibiting excellent high temperature shear performance and good adhesion to low surface energy substrates; 3. obtaining consistent performance over a broad UV curing range; 4. obtaining good through-cure for thick PSA films; and 5. reasonable cost to the general PSA market. Overcoming these challenges became the technical missions for our PSA research group in its plan to develop new and cost-effective UV curable PSAs for the high performance tape market. One of the leading UV PSA technologies is solvent-free acrylic syrup. The formation of an adhesive film involves subjecting to radiation in the near-UV region1 an acrylate-containing polymerizable mixture that includes monomers, oligomers, and/or polymers. This syrup technology can produce films with traditional PSA performance. However, the process requires protecting the syrup from oxygen (by flooding the curing line with nitrogen) and usually the curing speed is slow. Most important of all, this technology has been patented and used captively; therefore, it is not available to most tape manufacturers. A more recent development employs photoinitiators that are part of a polymerizable, organic structure. 2,3,4 In this way, the photoinitiator is covalently bound to the polymer backbone, ensuring cross-linking and chain branching rather than oligomer formation. This technology can be very effective in preventing the migration of the photoinitiator after coating and prior to irradiation, a common problem with non-polymeric initiators. However, the poor mobility of the initiator, a consequence of its large size, severely reduces efficiency of UV-initiated cross-linking. The result is
greatly reduced polymer cohesive strength. Finally, UV-initiated cationically cured epoxy systems can provide excellent PSA performance, but these products tends to suffer poor heat and moisture aging.5 The UV PSA technology developed by us employs the formation of an acrylated urethane hybrid, different from those previously reported and targeting improvement against all five of the described challenges. Experimental Methods Polymer formulation The acrylic urethanes formulation is performed at elevated temperatures after the urethane condensation polymerization has been completed. Film preparation The formulated UV PSAs can be made into PSA films according to the following method: the liquid products were preheated in the reservoir of a laboratory hot melt coater (Cheminstruments HLCL-1000) at approximately 110 C and coated onto a silicone release liner (LOPAREX RP 12). The film thickness was controlled by adjusting the gap between the coating bars. The coated adhesive films were then cured in air by UV irradiation using a laboratory UV curing line (Fusion DRS 120 NQ equipped with an H-bulb) at UV radiation dosages from 20 to 250 mJ/cm2. The UV exposure was measured using radiometers, either UVICURE Plus II from EIT-IM or ILT 393 from International Light. The cured film was finally laminated to one of three substrates: a release liner, Mylar film (PET), or Al metal film. The choice depended upon the performance test needs. The 2-mil solventborne adhesive films, used for comparison performance testing, were made in the lab by producing a drawdown, followed by 15 min air drying. The air dried films were cured in a 90!C oven for 5 minutes. The 5-mil solventborne adhesive films were prepared by overlaying two films that had been air dried and that produced 2.5 mil films after drying. These double-thickness films were then cured in a 90!C oven for 5 minutes. The heat cured films were then laminated to the appropriate substrate in the same manner as described above for UV PSA film. Adhesive performance test methods The cured films were evaluated by measurement of the peel, room temperature shear, and high temperature shear, using published adhesive tests6: Peel Adhesion-PSTC 101 Room Temperature Shear Resistance-PSTC-107 High temperature Shear Test Modified PSTC-107. A standard shear test with the panel hung in a temperature controlled 93!C and 150!C oven. Polymer Backbone Design and Synthesis It is well known that an inverse relationship usually exists between changes in adhesive and cohesive strength for a PSA product: loss of adhesion usually accompanies cohesion strength improvement, and vice versa. Therefore, significantly improving both adhesion and cohesion strengths for a PSA is a very
tough technical challenge. A new design for a polymer resin was necessary. The approach we took for the new polymer design included the choice of urethane-acrylate hybrid chemistry, design of a polymer with microstructure alternation, and careful optimization of the polymer molecular weight. Choice of the hybrid chemistry Among many polymer architectures considered, the marriage of an appropriately designed urethane backbone bearing pendant acrylate functionality was chosen. This backbone structure is known to offer excellent film flexibility and toughness. The primary challenges facing the use of urethane-acrylic hybrids in a pressure sensitive adhesive were improvement of high temperature shear resistance without sacrificing room-temperature performance, and compatibility towards a variety of adhesive additives, ensuring broad and straightforward formulation possibilities. Key raw material selection Several key factors were considered when choosing the raw material for the urethane polymerization:
1. Molecular weight 2. Compatibility with the reactant mixture 3. Polarity 4. Tg 5. Chemical stability (heat, weathering and others)
To avoid an impractically large experimental design, it was decided to focus the synthesis work based upon three principles: first, identify the use level for each key reactant; second, identify the proper molecular weight distribution so as to form a functional cross-link network and retain good coating properties; and third, optimize the product composition with respect to the compatibility between polymer and formulation components. A series of polymers were made and formulated into final products using several composition models based upon these principles. The result was a product that achieved excellent coatability, good adhesion and cohesion properties at room temperature, and excellent product composition compatibility.
Polymer microstructure alternation design The new polymer models selected from the above work showed some promising PSA performance features. However, the balance between room temperature and high temperature performance was not yet ideal. A different approach to solving this problem was taken: the adhesive characteristics were evaluated against changes in the microstructure of the polymer, while leaving the composition and molecular weight of the polymer unchanged. Several polymer structure models were built for this next study and their PSA performance characteristics are listed in Table I. All of the polymers are made with similar molecular weight. The compositions of the soft and the hard polymers are made with the same compositions as the soft and hard segments respectively in the invented polymer described in the Figure 1. The soft polymer model can offer excellent adhesion but lacks cohesive strength; the hard polymer model possesses excellent elasticity for cohesive strength but lacks adhesion and tack; the physical blend of soft and hard polymers offers excellent room temperature performance but could not provide acceptable high temperature performance. By contrast, the specially designed hybrid polymer made by purposely alternating the polymer microstructure with soft and hard segments offers balanced performance and superior individual performance in these standard adhesive tests.
Table 1. Polymer Structure versus PSA Performance
Performance Soft Hard Blend GMR 8020-02 93 C Shear, Kg/in2
(minutes) 9 151 166 >3000
30 min. Peel (lb/in) 4.07 1.39 4.35 4.35
Room Temp. Shear, 2 Kg/in2 (hours) 107 >